#------------------------------------------------------------------------------
#$Date: 2020-10-06 10:42:22 +0300 (Tue, 06 Oct 2020) $
#$Revision: 257415 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/55/73/1557378.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1557378
loop_
_publ_author_name
'Chen, Yan-Cong'
'Meng, Yan'
'Dong, Yan-Jie'
'Song, Xiao-Wei'
'Huang, Guo-Zhang'
'Zhang, Chuan-Lei'
'Ni, Zhao-Ping'
'Navařík, Jakub'
'Malina, Ondřej'
'Zbořil, Radek'
'Tong, Ming-Liang'
_publ_section_title
;
 Light- and temperature-assisted spin state annealing: accessing the
 hidden multistability
;
_journal_issue                   12
_journal_name_full               'Chemical Science'
_journal_page_first              3281
_journal_page_last               3289
_journal_paper_doi               10.1039/C9SC05971G
_journal_volume                  11
_journal_year                    2020
_chemical_formula_moiety         'C22 H14 Au2 Fe N6'
_chemical_formula_sum            'C22 H14 Au2 Fe N6'
_chemical_formula_weight         812.17
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2018-12-25
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2019-05-27 deposited with the CCDC.	2020-02-26 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 95.770(2)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.7739(5)
_cell_length_b                   13.9861(6)
_cell_length_c                   14.5762(7)
_cell_measurement_reflns_used    9752
_cell_measurement_temperature    80(2)
_cell_measurement_theta_max      27.49
_cell_measurement_theta_min      2.81
_cell_volume                     2185.28(17)
_computing_cell_refinement       'SAINT v8.37A (Bruker, 2015)'
_computing_data_reduction        'SAINT v8.37A (Bruker, 2015)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      80(2)
_diffrn_detector                 'CMOS active pixel sensor detector'
_diffrn_detector_type            'Bruker PHOTON 100 CMOS detector'
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device       'κ-geometry diffractometer'
_diffrn_measurement_device_type  'Bruker D8 QUEST'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  'mirror optics'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0462
_diffrn_reflns_av_unetI/netI     0.0185
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            66879
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.500
_diffrn_reflns_theta_min         2.677
_diffrn_source                   'microfocus sealed X-ray tube'
_diffrn_source_type              'Incoatec I\ms Microfocus'
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    14.070
_exptl_absorpt_correction_T_max  0.7456
_exptl_absorpt_correction_T_min  0.4437
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'SADABS-2014/5 (Bruker,2014/5) was used for absorption correction. wR2(int) was 0.1244 before and 0.0582 after correction. The Ratio of minimum to maximum transmission is 0.5951. The λ/2 correction factor is Not present.'
_exptl_crystal_colour            red
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    2.469
_exptl_crystal_description       block
_exptl_crystal_F_000             1488
_exptl_crystal_size_max          0.176
_exptl_crystal_size_mid          0.152
_exptl_crystal_size_min          0.144
_refine_diff_density_max         3.001
_refine_diff_density_min         -2.087
_refine_diff_density_rms         0.252
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.162
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     268
_refine_ls_number_reflns         4532
_refine_ls_number_restraints     60
_refine_ls_restrained_S_all      1.163
_refine_ls_R_factor_all          0.0499
_refine_ls_R_factor_gt           0.0391
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+69.6734P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0809
_refine_ls_wR_factor_ref         0.0865
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3762
_reflns_number_total             4532
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9sc05971g2.cif
_cod_data_source_block           80LS
_cod_depositor_comments
;Adding full bibliography for 1557376--1557379.cif.

 Adding full bibliography for 1557376--1557379.cif.
;
_cod_database_code               1557378
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.236
_shelx_estimated_absorpt_t_min   0.191
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Uiso/Uaniso restraints and constraints
Uanis(C17) \\sim Ueq, Uanis(C16) \\sim Ueq, Uanis(C15) \\sim Ueq, Uanis(C14)
\\sim Ueq, Uanis(N6) \\sim Ueq, Uanis(C22) \\sim Ueq, Uanis(C21) \\sim Ueq,
Uanis(C20) \\sim Ueq, Uanis(C19) \\sim Ueq, Uanis(C18) \\sim Ueq: with sigma of
0.005 and sigma for terminal atoms of 0.01
3.a Aromatic/amide H refined with riding coordinates:
 C5(H5), C7(H7), C8(H8), C9(H9), C10(H10), C12(H12), C13(H13), C14(H14),
 C17(H17), C18(H18), C19(H19), C16(H16), C21(H21), C22(H22)
3.b Fitted hexagon refined as free rotating group:
 C17(C18,C19,C20,C15,C16)
;
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Au1 Au 0.58276(3) 0.76568(3) 0.50762(2) 0.01556(10) Uani 1 1 d . . . . .
Au2 Au 0.69111(3) 0.26655(3) 0.54097(2) 0.01537(10) Uani 1 1 d . . . . .
Fe1 Fe 0.63285(11) 0.49953(10) 0.27355(9) 0.0108(2) Uani 1 1 d . . . . .
N1 N 0.6081(7) 0.6066(6) 0.3581(5) 0.0158(16) Uani 1 1 d . . . . .
N2 N 0.5844(7) 0.9154(6) 0.6669(6) 0.0177(17) Uani 1 1 d . . . . .
N3 N 0.6828(7) 0.4165(6) 0.3806(6) 0.0181(17) Uani 1 1 d . . . . .
N4 N 0.6631(7) 0.1068(6) 0.6889(5) 0.0164(17) Uani 1 1 d . . . . .
N5 N 0.8129(7) 0.5423(6) 0.2676(5) 0.0152(16) Uani 1 1 d . . . . .
N6 N 0.4532(8) 0.4544(6) 0.2782(6) 0.0248(19) Uani 1 1 d . U . . .
C1 C 0.5983(8) 0.6670(8) 0.4104(7) 0.019(2) Uani 1 1 d . . . . .
C2 C 0.5772(8) 0.8613(7) 0.6075(7) 0.0170(19) Uani 1 1 d . . . . .
C3 C 0.6945(8) 0.3631(7) 0.4410(7) 0.019(2) Uani 1 1 d . . . . .
C4 C 0.6794(9) 0.1662(7) 0.6381(6) 0.0168(19) Uani 1 1 d . . . . .
C5 C 0.8581(8) 0.5500(6) 0.1871(7) 0.0153(18) Uani 1 1 d . . . . .
H5 H 0.804436 0.535842 0.133045 0.018 Uiso 1 1 calc R . . . .
C6 C 0.9818(8) 0.5781(7) 0.1767(7) 0.0164(19) Uani 1 1 d . . . . .
C7 C 1.0250(9) 0.5854(8) 0.0886(7) 0.024(2) Uani 1 1 d . . . . .
H7 H 0.969280 0.573855 0.035028 0.029 Uiso 1 1 calc R . . . .
C8 C 1.1460(10) 0.6090(8) 0.0799(8) 0.031(3) Uani 1 1 d . . . . .
H8 H 1.175077 0.612784 0.020626 0.037 Uiso 1 1 calc R . . . .
C9 C 1.2278(9) 0.6277(7) 0.1598(8) 0.027(2) Uani 1 1 d . . . . .
H9 H 1.311698 0.645323 0.153655 0.032 Uiso 1 1 calc R . . . .
C10 C 1.1887(9) 0.6210(7) 0.2453(7) 0.021(2) Uani 1 1 d . . . . .
H10 H 1.245774 0.632977 0.298067 0.026 Uiso 1 1 calc R . . . .
C11 C 1.0644(9) 0.5964(7) 0.2566(7) 0.021(2) Uani 1 1 d . . . . .
C12 C 1.0139(9) 0.5881(7) 0.3417(7) 0.023(2) Uani 1 1 d . . . . .
H12 H 1.065172 0.600723 0.397291 0.027 Uiso 1 1 calc R . . . .
C13 C 0.8926(9) 0.5624(7) 0.3454(7) 0.021(2) Uani 1 1 d . . . . .
H13 H 0.861555 0.558017 0.404021 0.025 Uiso 1 1 calc R . . . .
C14 C 0.3838(12) 0.4203(10) 0.2036(10) 0.043(3) Uani 1 1 d . U . . .
H14 H 0.412478 0.417031 0.144194 0.052 Uiso 1 1 calc R . . . .
C17 C 0.0589(8) 0.3248(7) 0.1589(6) 0.056(4) Uani 1 1 d . U . . .
H17 H 0.006044 0.302398 0.107304 0.067 Uiso 1 1 calc R . . . .
C18 C 0.0158(7) 0.3272(7) 0.2456(7) 0.058(4) Uani 1 1 d G U . . .
H18 H -0.066558 0.306489 0.253254 0.069 Uiso 1 1 calc R . . . .
C19 C 0.0931(9) 0.3599(8) 0.3212(5) 0.058(4) Uani 1 1 d G U . . .
H19 H 0.063603 0.361574 0.380466 0.069 Uiso 1 1 calc R . . . .
C20 C 0.2135(8) 0.3902(7) 0.3101(5) 0.045(3) Uani 1 1 d G U . . .
C15 C 0.2567(6) 0.3878(7) 0.2234(6) 0.046(3) Uani 1 1 d G U . . .
C16 C 0.1793(8) 0.3551(7) 0.1478(5) 0.053(4) Uani 1 1 d G U . . .
H16 H 0.208812 0.353393 0.088565 0.064 Uiso 1 1 calc R . . . .
C21 C 0.2884(14) 0.4273(11) 0.3813(11) 0.051(4) Uani 1 1 d . U . . .
H21 H 0.262046 0.432672 0.441379 0.061 Uiso 1 1 calc R . . . .
C22 C 0.4033(11) 0.4566(9) 0.3622(9) 0.038(3) Uani 1 1 d . U . . .
H22 H 0.455913 0.481729 0.412704 0.045 Uiso 1 1 calc R . . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -2.0133 8.8022 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C1 Au1 Au2 83.1(3) . 3_666 ?
C2 Au1 Au2 100.0(3) . 3_666 ?
C2 Au1 C1 176.6(4) . . ?
C3 Au2 Au1 91.1(3) . 3_666 ?
C3 Au2 C4 176.9(4) . . ?
C4 Au2 Au1 86.1(3) . 3_666 ?
N1 Fe1 N2 89.6(3) . 4_575 ?
N1 Fe1 N3 89.8(3) . . ?
N1 Fe1 N4 178.2(3) . 4_565 ?
N1 Fe1 N5 89.6(3) . . ?
N1 Fe1 N6 91.5(3) . . ?
N2 Fe1 N5 88.1(3) 4_575 . ?
N2 Fe1 N6 92.0(3) 4_575 . ?
N3 Fe1 N2 179.1(4) . 4_575 ?
N3 Fe1 N4 90.1(3) . 4_565 ?
N3 Fe1 N5 91.2(3) . . ?
N3 Fe1 N6 88.6(3) . . ?
N4 Fe1 N2 90.5(3) 4_565 4_575 ?
N4 Fe1 N5 88.7(3) 4_565 . ?
N4 Fe1 N6 90.3(3) 4_565 . ?
N5 Fe1 N6 178.9(4) . . ?
C1 N1 Fe1 176.6(8) . . ?
C2 N2 Fe1 168.3(7) . 4_576 ?
C3 N3 Fe1 170.0(8) . . ?
C4 N4 Fe1 178.0(8) . 4_566 ?
C5 N5 Fe1 119.9(6) . . ?
C5 N5 C13 117.4(8) . . ?
C13 N5 Fe1 122.7(6) . . ?
C14 N6 Fe1 122.3(9) . . ?
C14 N6 C22 119.2(11) . . ?
C22 N6 Fe1 118.4(8) . . ?
N1 C1 Au1 176.3(9) . . ?
N2 C2 Au1 174.3(8) . . ?
N3 C3 Au2 172.4(8) . . ?
N4 C4 Au2 174.0(8) . . ?
N5 C5 C6 123.7(9) . . ?
C5 C6 C7 121.2(9) . . ?
C5 C6 C11 118.9(9) . . ?
C7 C6 C11 119.8(9) . . ?
C8 C7 C6 120.5(10) . . ?
C7 C8 C9 119.4(10) . . ?
C10 C9 C8 121.2(9) . . ?
C9 C10 C11 120.7(10) . . ?
C10 C11 C6 118.3(9) . . ?
C10 C11 C12 125.4(10) . . ?
C12 C11 C6 116.3(9) . . ?
C13 C12 C11 120.9(9) . . ?
C12 C13 N5 122.7(9) . . ?
N6 C14 C15 113.4(12) . . ?
C18 C17 C16 120.0 . . ?
C19 C18 C17 120.0 . . ?
C18 C19 C20 120.0 . . ?
C19 C20 C15 120.0 . . ?
C21 C20 C19 121.3(9) . . ?
C21 C20 C15 118.6(9) . . ?
C20 C15 C14 124.3(8) . . ?
C16 C15 C14 115.7(8) . . ?
C16 C15 C20 120.0 . . ?
C15 C16 C17 120.0 . . ?
C20 C21 C22 116.3(14) . . ?
C21 C22 N6 128.0(13) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Au1 Au2 2.9984(5) 3_666 ?
Au1 C1 1.997(11) . ?
Au1 C2 1.982(10) . ?
Au2 C3 1.990(10) . ?
Au2 C4 2.007(10) . ?
Fe1 N1 1.974(8) . ?
Fe1 N2 1.985(9) 4_575 ?
Fe1 N3 1.976(9) . ?
Fe1 N4 1.981(8) 4_565 ?
Fe1 N5 2.041(8) . ?
Fe1 N6 2.044(9) . ?
N1 C1 1.150(13) . ?
N2 C2 1.148(13) . ?
N3 C3 1.152(13) . ?
N4 C4 1.138(12) . ?
N5 C5 1.320(12) . ?
N5 C13 1.381(12) . ?
N6 C14 1.344(16) . ?
N6 C22 1.386(15) . ?
C5 C6 1.412(12) . ?
C6 C7 1.413(14) . ?
C6 C11 1.416(14) . ?
C7 C8 1.363(14) . ?
C8 C9 1.413(16) . ?
C9 C10 1.358(15) . ?
C10 C11 1.408(14) . ?
C11 C12 1.409(15) . ?
C12 C13 1.362(14) . ?
C14 C15 1.498(15) . ?
C17 C18 1.3900 . ?
C17 C16 1.3900 . ?
C18 C19 1.3900 . ?
C19 C20 1.3900 . ?
C20 C15 1.3900 . ?
C20 C21 1.353(17) . ?
C15 C16 1.3900 . ?
C21 C22 1.359(18) . ?
